Cu~3~Sn - understanding the systematic absences.
Müller, Carola J; Lidin, Sven; Acta Crystallographica, Section B: Structural Science, Crystal Engineering and Materials 70 (2014) 879–887; doi:10.1107/S205252061401806X

data_2310772
_publ_section_title
;
 Cu~3~Sn - understanding the systematic absences.
;
_journal_coden_ASTM              ACSBDA
_journal_coeditor_code           DQ5008
_journal_issue                   5
_journal_name_full
;
 Acta Crystallographica, Section B: Structural Science, Crystal Engineering
 and Materials
;
_journal_page_first              879
_journal_page_last               887
_journal_paper_doi               10.1107/S205252061401806X
_journal_volume                  70
_journal_year                    2014
_chemical_formula_structural     'Cu3 Sn1'
_chemical_formula_sum            'Cu3 Sn'
_chemical_formula_weight         309.3
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   5.51960(10)
_cell_length_b                   38.2386(12)
_cell_length_c                   4.33210(10)
_cell_measurement_reflns_used    2178
_cell_measurement_temperature    293
_cell_measurement_theta_max      28.38
_cell_measurement_theta_min      3.2
_cell_volume                     914.34(4)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.32 (release 02-08-2013 CrysAlis171 .NET)
(compiled Aug  2 2013,16:46:58)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.32 (release 02-08-2013 CrysAlis171 .NET)
(compiled Aug  2 2013,16:46:58)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.32 (release 02-08-2013 CrysAlis171 .NET)
(compiled Aug  2 2013,16:46:58)
;
_diffrn_ambient_temperature      293
_diffrn_detector_area_resol_mean 16.1367
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.97
_diffrn_measurement_device       'four-cycle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos'
_diffrn_measurement_method       '\w and \p scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'Enhance (Mo) X-ray Source'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.0341
_diffrn_reflns_av_unetI/netI     0.0124
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       50
_diffrn_reflns_limit_k_min       -49
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            7324
_diffrn_reflns_theta_full        28.17
_diffrn_reflns_theta_max         28.38
_diffrn_reflns_theta_min         3.2
_exptl_absorpt_coefficient_mu    37.885
_exptl_absorpt_correction_T_max  0.529
_exptl_absorpt_correction_T_min  0.095
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.32 (release 02-08-2013 CrysAlis171 .NET)
(compiled Aug  2 2013,16:46:58)
Analytical numeric absorption correction using a multifaceted crystal
   model based on expressions derived by R.C. Clark & J.S. Reid.
(Clark, R. C. & Reid, J. S. (1995). Acta Cryst. A51, 887-897)
;
_exptl_crystal_colour            'metallic intense silver'
_exptl_crystal_density_diffrn    8.986
_exptl_crystal_description       block
_exptl_crystal_F_000             2192
_exptl_crystal_size_max          0.142
_exptl_crystal_size_mid          0.051
_exptl_crystal_size_min          0.018
_refine_diff_density_max         1.34
_refine_diff_density_min         -1.25
_refine_ls_extinction_coef       225(12)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    2.54
_refine_ls_goodness_of_fit_ref   1.96
_refine_ls_number_constraints    0
_refine_ls_number_parameters     58
_refine_ls_number_reflns         689
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0419
_refine_ls_R_factor_gt           0.0256
_refine_ls_shift/su_max          0.0485
_refine_ls_shift/su_mean         0.0081
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(\s^2^(I)+0.0004I^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0904
_refine_ls_wR_factor_ref         0.0965
_reflns_number_gt                389
_reflns_number_total             689
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            dq5008sup1.cif
_cod_data_source_block           673K-superstructure
_cod_original_sg_symbol_Hall     '-C -2x;-2yc;-2zc'
_cod_original_formula_sum        'Cu3 Sn1'
_cod_database_code               2310772